- Photo-oxidation of polymers
Photo-oxidation is the oxidation of a polymer surface in the presence of oxygen or ozone that is facilitated radiant energy such as UV or artificial light. This proces is often the the most significant component of weather degradation of polymers. Photo-oxidation results in chemical changes and normally a reduction in the polymer's molecular weight. Consequently, the material becomes more brittle coinciding with a reduction in tensile strength, impact strength, elongation at break. Often discoloration and loss of gloss accompany photo-oxidaiton. High temperature and stress concentration are significant factors to increase reaction rate of photo-oxidation.
General mechanism of polymer photo-oxidation
In the photo-oxidation reaction including chain scission, cross linking and secondary oxidative reactions, the following step can be considered:Rabek, JF 1990, Photostabilization of Polymers:Principles and Application, ELSEVIER SCIENCE PUBLISHER LTD, England]
#Initial step: Free radical formation can be formed by light absorption.
#Chain Propagation step: The free radical reacts with oxygen to produce polymer peroxy radicals (POO•) and generate polymer hydroperoxide (POOH) and new polymer alkyl radical (P•).
#Chain Branching: The formation of polymer oxy radicals (PO•) and hydroxy radicals (HO•) can be formed by photolysis.
#Termination step: Cross linking is a result of the reaction of different free radicals with each other.
P• = Polymer alkyl radical
PO• = Polymer oxy radical (Polymer alkoxy radical)
POO• = Polymer peroxy radical (Polymer alkylperoxy radical)
POOH = Polymer hydroperoxide
HO• = hydroxy radical
Aldehydes, ketones and carboxylic acids either along or at the end of polymer chains are generated by oxygenated species in photolysis of photo-oxidation. The major need to occur initiation of photo-oxidation reactions is the existence of chromophoric groups in the macromolecules. Generally photo-oxidation, however, can occur simultaneously with thermal degradation and one of these can accelerate another.
Adding pigment light absorbers and photostabilizer known as UV absorbers are the ways to protect photo-oxidation in polymers. Antioxidants are another prominent method to inhibit the formation of hydroperoxides in photo-oxidation process.
Effects of dyes/pigments
Dyes and pigments are used in polymer materials to give color changing properties. These additives can change the stability against degradation. Such as Cu-phthalocyanine dye can stabilize against degradation and as well as accelerate degradation in other situations. Cu-phthalocyanine incorporated into polycarbonate (PC) results in an acceleration of the degradation when subjected to photochemical aging. This is based on the idea that PC containing Cu-phthalocyanine where specific interactions among the excited states of PC and Cu-phthalocyanine take place and enhance the formation of relative species in PC. The excited Cu-phthalocyanine may abstract hydrogen atoms from methyl groups in the PC, which increase the formation of free radicals that act as the starting points for the sequential photo-oxidation reactions that lead to the degradation of the PC. Also electron transfer sensitization is another possible mechanism where the excited Cu-phthalocyanine abstracts electrons from PC to form Cu-Ph radical anion and PC radical cations. These species in presence of oxygen can cause oxidation of the aromatic ring. [Clodoaldo Saron, Fabio Zulli, Marco Giordano, Maria Isabel Felisberti, Influence of copper-phthalocyanine on the photodegradation of polycarbonate, Polymer Degradation and Stability, Volume 91, Issue 12, December 2006, Pages 3301-3311]
Protection against photo-oxidation
Poly(ethylene-naphthalate) (PEN) can be protected by applying zinc oxide coating, this film acts a protective layer where it reduces the diffusion of oxygen with PEN. [L. Guedri-Knani, J. L. Gardette, M. Jacquet, A. Rivaton, Photoprotection of poly(ethylene-naphthalate) by zinc oxide coating, Surface and Coatings Technology, Volumes 180-181, 1 March 2004, Pages 71-75] Zinc oxide can also be used on polycarbonate (PC) where often used in outdoor applications. Again the zinc oxide can protect PC form solar radiation and decrease the oxidation rate and photo-yellowing of PC. [A. Moustaghfir, E. Tomasella, A. Rivaton, B. Mailhot, M. Jacquet, J. L. Gardette, J. Cellier, Sputtered zinc oxide coatings: structural study and application to the photoprotection of the polycarbonate, Surface and Coatings Technology, Volumes 180-181, 1 March 2004, Pages 642-645.]
*Grassie, N & Scott, G 1985, Polymer Degradation Stabilisation, Press Syndicate of University of Cambridge, England
*Schnabel, W 1981, Polymer Degradation: Principles and Pratical Applications, Macmillan Publishing Co., Inc, New York
*Photo-Oxidation, accessed 22/04/08, http://www.ozonelab.com/glossary/p/photo-oxidation.htm
forensic polymer engineering
Wikimedia Foundation. 2010.
Look at other dictionaries:
Stabilizers for polymers — are used directly or by combinations to prevent the various effects such as oxidation, chain scission and uncontrolled recombinations and cross linking reactions that are caused by photo oxidation of polymers. Polymers are considered to get… … Wikipedia
Thermal degradation of polymers — is molecular deterioration as a result of overheating. At high temperatures the components of the long chain backbone of the polymer can begin to separate (molecular scission) and react with one another to change the properties of the polymer.… … Wikipedia
Chemically Assisted Degradation of Polymers — is a type of polymer degradation that involves a change of the polymer properties due to a chemical reaction with the polymer’s surroundings. There are many different types of possible chemical reactions causing degradation however most of these… … Wikipedia
Chemically assisted degradation of polymers — is a type of polymer degradation that involves a change of the polymer properties due to a chemical reaction with the polymer’s surroundings. There are many different types of possible chemical reactions causing degradation however most of these… … Wikipedia
Polymer degradation — is a change in the properties tensile strength, colour, shape, etc of a polymer or polymer based product under the influence of one or more environmental factors such as heat, light or chemicals. These changes are usually undesirable, such as… … Wikipedia
Polyphenol — Plant derived polyphenol, tannic acid, formed by esterification of ten equivalents of the phenylpropanoid derived gallic acid to a monosaccharide (glucose) core from primary metabolism … Wikipedia
Antioxidant — Model of the antioxidant metabolite glutathione. The yellow sphere is the redox active sulfur atom that provides antioxidant activity, while the red, blue, white, and dark grey spheres represent oxygen, nitrogen, hydrogen, and carbon atoms,… … Wikipedia
Photoconductive atomic force microscopy — (pc AFM) is a scientific technique.. Multi layer photovoltaic cells have gained popularity since mid 1980s. At the time, research was primarily focused on single layer photovoltaic (PV) devices between two electrodes, in which PV properties… … Wikipedia
Phalloidin — Chembox new ImageFile=Phalloidin.png ImageSize=200px IUPACName= OtherNames= Section1= Chembox Identifiers CASNo=17466 45 4 PubChem=441542 SMILES= Section2= Chembox Properties Formula=C35H48N8O11S MolarMass=788.87 g/mol Appearance= Density=… … Wikipedia
Ultraviolet — UV redirects here. For other uses, see UV (disambiguation). UVB redirects here. For the mysterious shortwave radio station in Russia, see UVB 76. For other uses, see Ultraviolet (disambiguation). False color image of the Sun s corona as seen in… … Wikipedia